Perovskite-type organic-inorganic hybrid NLO switches tuned by guest cations
Fu-Juan Geng; Lin Zhou; Ping-Ping Shi; Xiao-Li Wang; Xuan Zheng; Yi Zhang; Da-Wei Fu; Qiong Ye; Journal of Materials Chemistry C 5 (2017) 1529–1536; doi:10.1039/C6TC05105G

data_7235184
_publ_section_title
;
 Perovskite-type organic-inorganic hybrid NLO switches tuned by guest
 cations
;
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              1529
_journal_page_last               1536
_journal_paper_doi               10.1039/C6TC05105G
_journal_volume                  5
_journal_year                    2017
_chemical_formula_moiety         'C6 Mn N9,C9 H20 P'
_chemical_formula_sum            'C15 H20 Mn N9 P'
_chemical_formula_weight         412.31
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_cell_angle_alpha                90
_cell_angle_beta                 96.32(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.098(2)
_cell_length_b                   12.156(2)
_cell_length_c                   17.119(3)
_cell_measurement_reflns_used    3275
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.1643
_cell_measurement_theta_min      1.7642
_cell_volume                     2088.6(7)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.986
_diffrn_measured_fraction_theta_max 0.967
_diffrn_measurement_device_type  'Saturn724+ (4x4 bin mode)'
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0324
_diffrn_reflns_av_unetI/netI     0.0329
_diffrn_reflns_Laue_measured_fraction_full 0.986
_diffrn_reflns_Laue_measured_fraction_max 0.967
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            14170
_diffrn_reflns_point_group_measured_fraction_full 0.986
_diffrn_reflns_point_group_measured_fraction_max 0.967
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.481
_diffrn_reflns_theta_min         3.305
_exptl_absorpt_coefficient_mu    0.726
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    1.311
_exptl_crystal_description       Prism
_exptl_crystal_F_000             852
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.200
_exptl_crystal_size_min          0.200
_refine_diff_density_max         0.603
_refine_diff_density_min         -0.384
_refine_diff_density_rms         0.058
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     238
_refine_ls_number_reflns         4636
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.061
_refine_ls_R_factor_all          0.0615
_refine_ls_R_factor_gt           0.0484
_refine_ls_shift/su_max          0.010
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0629P)^2^+1.2616P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1234
_refine_ls_wR_factor_ref         0.1319
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                3786
_reflns_number_total             4636
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            J-Mater-Chem-C-2017-5-1529.cif
_cod_data_source_block           1
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               7235184
_shelx_estimated_absorpt_t_min   0.868
_shelx_estimated_absorpt_t_max   0.868
_shelx_res_checksum              35038